This research investigates the mechanical shear behavior of twelve reinforced concrete beams. The type of loading (normal or reverse), the
pres-ence or abspres-ence of steel ibers (30 kgf/m3_{), and the concrete compressive strength (40MPa, 60 MPa, or 80 MPa) were the mains test variables }
studied. The beams had nominally identical cross-sections, effective depths, and longitudinal and transverse reinforcements. The loads were
increased at 10 kN intervals until shear failure occurred, deined by the yielding of the irst stirrup. The ultimate shear loads observed in these
tests were compared to three empirical and semi-empirical formulas proposed in the literature. Based on the test results it could be concluded that
concrete compressive strength has no signiicant inluence on the reduction of ultimate shear load caused by reverse loading. Reverse-loaded
beams with ibers had approximately the same ultimate shear strength as concrete beams without ibers subjected to normal loading, regardless
of the compressive strength of the concrete.

* Keywords*: steel iber; reinforced concrete; beam; reverse loading; shear strength.

Este trabalho investiga o comportamento ao esforço cortante de doze vigas em concreto com adição de ibras de aço. As principais variáveis estudadas foram o tipo de carregamento (normal ou reverso), a presença ou a ausência de ibras de aço (30kgf/m³) e a resistência do concreto à compressão (40 MPa, 60 MPa, ou 80 MPa). As vigas apresentavam seção transversal, altura útil e armaduras longitudinais e transversais nominalmente idênticas. Uma carga concentrada, no meio do vão da viga, foi aplicada em intervalos de 10 kN até a ruptura por cisalhamento, deinida pelo escoamento do primeiro estribo em solicitação. A carga última de cisalhamento observada nos testes foi comparada com três for -mulas empíricas, e semi-empiricas, propostas na literatura. Baseando-se nos resultados dos testes, concluiu-se que a resistência à compressão do concreto não tem inluencia signiicativa na parcela de redução da carga ultima de cisalhamento, promovida pela reversão do carregamento. Vigas sujeitas ao carregamento reverso e com ibras apresentaram, aproximadamente, a mesma resistência última de cisalhamento que as vigas sem ibras sujeitas ao carregamento normal, independentemente da resistência do concreto à compressão.

* Palavras-chave: *ibras de aço; concreto armado; viga; carregamento reverso; resistência ao cisalhamento.

**The shear strength of steel iber-reinforced **

**concrete beams**

**Resistência ao cisalhamento de vigas de concreto **

**Resistência ao cisalhamento de vigas de concreto**

**reforçado com ibras de aço**

**reforçado com ibras de aço**

**A. L. MORENO JUNIOR a**
almoreno@fec.unicamp.br

**A. P. VEDOATO b**

ana.vedoato@yahoo.com.br

*a _{ Faculdade de Engenharia Civil, Arquitetura e Urbanismo, Departamento de Estruturas, Unicamp, almoreno@fec.unicamp.br, Av. Albert Einstein, 951 - }*

*Caixa Postal: 6021 - CEP: 13083-852, Campinas, Brazil*

*b _{ Faculdade de Engenharia Civil, Arquitetura e Urbanismo, Departamento de Estruturas, Unicamp, ana.vedoato@yahoo.com.br, Av. Albert Einstein, 951 }*

*- Caixa Postal: 6021 - CEP: 13083-852, Campinas, Brazil*

*Received: 19 Aug 2010 • Accepted: 03 Oct 2011 • Available Online: 28 Nov 2011*

**Abstract **

**1. Introduction**

Many studies have investigated the shear behavior of steel iber reinforced concrete beams (Araúz [3]; Ashour et al. [4]; Cucchi-ara et al. [5]; Di Prisco and Romero [6]; Furlan Jr and de Hanai [7]; Parra-Montesinos [16], Swamy and Bahla [19]; Swamy and Balla [20]). Some authors have considered placing the burden of shear reinforcement on the ibers and several have found that add-ing steel ibers to a reinforced concrete beam increases its shear strength. Furthermore, a suficient amount of ibers can suppress brittle shear failure in favor of more ductile behavior. The increase in shear strength depends not only on the amount of ibers, usually expressed as a fraction of the beam volume, but also on their aspect ratio and anchorage conditions. The ibers decrease the crack open -ing displacement and promote so-called alternative shear strength mechanisms, especially aggregate interlock and dowel action. Narayanan and Darwish [11]; [12] observed that iber-reinforced concrete beams and reinforced concrete beams with conventional stirrups devel-op similar crack patterns under very high shear stress, and concluded that ibers cannot entirely replace conventional shear reinforcement. Several empirical expressions and analytical models have been proposed to evaluate the contribution of ibers to the ultimate shear strength (Mansur et al. [9]; Narayanan and Darwish [11]; Noghabai [13]; Oh and Lim [14]; Tan et al. [22]). This contribution depends mainly on three factors: the volume fraction of the ibers, the shape of the ibers, and the nature of the iber-matrix interface. (The last one determines the resistance of the ibers to pullout.) However, no existing expression has yet been validated by a wide range of tests. In some cases, the calibration data even include the beams that failed by lexure or even by shear. The design procedures pro -posed for estimating shear strength need to be evaluated using a large collection of test results from beams that failed in shear. However, only a few studies contain experimental data about shear be -havior of iber-reinforced beams submitted to reverse loadings, or even beams with conventional transverse reinforcement (Oliveira [15]; Paulay [17]; Wang et al. [23]). Paulay [17]) found that under reverse loadings, new cracks formed at an intersecting diagonal by cracks created during the previous loading (an example of this appears later in the paper). In this context, cracks covered the entire compression zone at the top of the beam and the residual deformation of the longitudinal reinforcement pre-vents the cracks to be fully closed. Thus, compared to a normal loading, the compression chord and aggregate interlock of a beam subjected to reverse loadings may contribute much less to the ultimate shear strength. Recent studies carried out at the University of Campinas (Oliveira [15]) conirmed that reversion has an unfavorable effect on the shear resistance of reinforced concrete beams. In these experi-ments, the application of a reverse load reduced the ultimate shear strength of concrete beams by at least 50 per cent.

Design codes seldom consider alternative mechanisms (aggregate interlock, dowel action, arch action) to calculate the shear strength of reinforced concrete beams (e.g., ACI Committee 318 [2]). In some cases, they do not even refer the procedures for estimating the shear strengths of beams submitted to reverse loadings. The reverse loading decreases the ultimate shear strength of rein-forced concrete beams and adding the steel ibers increase its capac-ity. It stands to reason that a concrete beam with steel ibers could sustain reverse loads comparable to the normal shear loads sus-tained by normal concrete beams. This paper describes experimental

measurements of reinforced concrete beams with steel ibers submit -ted to reverse shear loading. The ultimate shear loads recorded ex-perimentally will also be compared to semi-empirical expressions pro-posed by Al-Taán & Al-Feel [1], Swamy et al. [21], and Sharma [18].

**2. Materials and experimental program**

**2.1 Test program**

**2.1 Test program**

These experiments test concrete beams of various compressive
strengths (40 MPa, 60 MPa and 80 Mpa), both with and without steel
ibers, under normal and reverse loading. Thus, each compressive
strength test required four different tests, for a total of twelve beams.
The beam designations consist of several terms: an initial letter
“I” (their cross-sectional form), the nominal concrete compressive
strength in MPa, the steel carbon content (BC for low content and
AC for high content), the amount of steel ibers (zero or 30 kg of iber
per m3_{ of concrete), and the type of loading (N for normal or I for re}_{}

-verse). Beam I-80-BC30-I, for instance, has strength of 80 MPa and steel ibers of low carbon content. The amount of ibers was 30 kgf per cubic meter, and the beam experienced reverse loading. The cross-sectional dimensions, effective depths, and longitudi-nal and transverse reinforcements of the beams were nomilongitudi-nally identical. The areas of longitudinal and shear reinforcement were designed to obtain a premature shear failure; therefore, a stirrup always yields before a longitudinal reinforcement.

The beam specimens were 1800 mm long with the span length of
1550 mm and simply supported at both ends. A point load was applied
at midspan in all specimens. The shear span *a* was 775 mm and the
effective depth *d* was 178 mm, so the ratio *a*/*d* was 4.12 in all cases.
The longitudinal reinforcement consisted of six steel bars with
di-ameters of 16.0 mm: three in the top layer and three in the bottom
layer (ρ_{l }= 3.12%). The shear reinforcement consisted of vertical
stirrups with diameters of 4.2 mm, spaced 15 centimeters apart
(ρ_{w}=3.12%). Figure [1] shows the dimensions of the beams.

Linear Variable Delection Transducers (LVDT) measured out-of-plane delections at midspan. The strain gauges, LVDTs and load cells were connected to a computerized data acquisition system and the data were taken in the range of one second during loading. For all beams, we observed and recorded the crack pattern after each load increment. The load was increased until shear failure occurred, meaning that a stirrup yielded while the longitudinal rein-forcements remained intact.

**2.3 Material properties**

**2.3 Material properties**

The concrete was made with Type I Portland cement. The coarse aggregates were crushed gravel with a maximum size of 19 mm and modulus of ineness (MF) of 6.23. The ine aggregates were natural river sand with a MF of 2.24. The addition of water-reducing admixture and silica fume (amount of 10% of the cement mass), improved the workability of the higher-strength concrete.

The low-carbon steel hooked iber had length Lf = 60 mm,

equiva-lent diameter Df = 0.8 mm (aspect ratio Lf /Df = 66.7), and a nominal

tensile strength of 1115 MPa. The amount of steel ibers was 30
kgf/m3_{ (v}

f = 0.4%) in each beam that contain them.

To better understand the behavior of the compressive strength and deformation capacity of the plain and fibrous concrete, six cylindrical specimens of each type with diameter 100 mm and height 200 mm were taken simultaneously with the preparation of the beams, permitting three independent tests of each prop-erty. The samples were covered with wet burlap and plastic foil for one week, then unwrapped and tested at 28 days old. Table [1] reports the mix designs and measured strengths of the three concretes.

**2.2 Test arrangment**

**2.2 Test arrangment**

A hydraulic jack of 500 kN capacity applied the loads through a rectan -gular plate attached to the beam. A load cell measured the real applied loads. In cases without reversion, only one of the chords received the load. The loads were applied through the jack with an increment of 10 kN until a shear failure occurred. For loading reversion cases, the jack was applied to both chords alternately in increments of 10 kN (i.e., 10 kN, 10 kN reversed, 20 kN, 20 kN reversed, and so on).

Electrical resistance strain gauges monitored strain in the steel. Each beam had strain gauges on eight stirrups (T1 up to T8) at middle height. Six extensometers were placed at midspan (L1 up to L6) along the longitudinal reinforcing bars, three in the top layer and three in the bottom layer. Two extensometers were also placed in the central bar, one on the top layer and one on the lower layer, placed at a distance equivalent to 1/4 of the beam span in relation to the support (L7 up to L10). Figure [2] illustrates the instrumenta -tion of the longitudinal reinforcements and stirrups.

### Figure 2 – Instrumentation of Beams

### Table 1 – Experimental mixtures

### Mixture

### Series 1

### Series 2

### Series 3

3

### CEMENT (kg/m )

### 656

### 350

### 656

3

### SILICA FUME (kg/m )

### 66

### ---

### 66

3

### FINE AGREGATE (kg/m )

### 808

### 820

### 808

### COARSE AGGREGATE

3### (kg/m )

### 1234

### 1040

### 1234

3

### WATER (l/m )

### 182

### 198

### 230

### SUPERPLASTICIZER

3### (l/m )

### 27.5

### ----

### 27.5

3

### STEEL FIBERS (kgf/m )

### 0 - 30

### 0 - 30

### 0 - 30

### w/c (WATER/CEMENT)

### (l/kgf)

### 0.29

### 0.59

### 0.35

### ¦

### ´c (MPa)

### 82.0 - 80.1

### 41.2 - 40.3

### 60.5 - 63.1

for iber-reinforced concrete beams and

### (5)

### V

u### = V

c### + V

s### - V

rfor beams without ibers.

**3. Results and discussions**

**3.1 Cracking**

**3.1 Cracking**

Initial lexure cracks always were formed along the bottom chord at midspan. The cracks had been regularly spaced, and their length increased when the load increased. Later, shear cracks formed near the quarter-span point. The beams eventually failed along a single shear crack.

In cases of reverse loading, two intersecting shear crack patterns were formed (Figure [3]).

**3.2 Web reinforcement**

**3.2 Web reinforcement**

All beams failed by shear and their ultimate shear loads corre-spond to the irst load when a stirrup yielded. In all cases this oc-curred before any longitudinal reinforcement yielded.

Figures [4], [5], and [6] plot the shear force, V (F/2), versus stirrup
stress, σ* _{sw}*, for each series. The stress data come from the most
solicited stirrup on each beam.

Figures [7] and [8] show the same data for normally loaded and reverse loaded beams, comparing the beams of different compres-sive strengths.

In all cases, under small loads, the stirrup stress increases very slowly and the classical truss analogy is not relevant. The truss model is valid only after the beams begin cracking and the web reinforcement starts to tension. In that case, the Based on tension coupon tests, the average modulus of elasticity,

yield strength and speciic yielding deformation of the longitudinal bars were 201 GPa, 573 MPa and 0.29% respectively.

The average modulus of elasticity, yield strength and speciic yield-ing deformation of the vertical stirrups (web reinforcement) were 201 GPa, 682 MPa and 0.54% respectively. The web reinforce-ment ratio was 0.37%.

**2.4 Shear strenght of steel iber-reinforced **

**2.4 Shear strenght of steel iber-reinforced**

**concrete beams and the truss mechanism **

For shear design purposes, the parallel chord truss is analogous to
a web-reinforced concrete beam. First postulated by Mörsch [10],
this old concept (the classical truss analogy) calls for stirrups as
tension members and concrete struts running parallel to diagonal
cracks, generally at 45 degrees to the beam axis. The lexural
con-crete compression zone and the lexural reinforcement form the
top and bottom chords of the analogous pin-jointed truss and the
equilibrium considerations are sufice to determine the forces in
the truss. The predicted ultimate shear force V**concrete beams and the truss mechanism**

_{u}is equivalent to the maximum shear force Vs sustainable by the web reinforcement:

### (1)

### V

u### = Vs

### =

### r

w yw### f bd

where *d* is the effective depth, *b* is the beam width, ƒ_{yw} is the web
reinforce-ment yield strength, and ρ_{w} is the steel ratio of the web reinforcement.
In experiments observing the stirrup load-stress behavior of concrete
beams, Leonhardt and Walther [8] assumed that the web reinforce
-ments bear only part of the ultimate shear load. A number of
“alter-native” mechanisms (aggregate interlock, longitudinal reinforcement
dowel action, arch action) provide additional resistance, so the
ulti-mate shear load should be expressed mathematically as follows:

### (2)

### V

u### = Vc

### + V

swhere V_{s} is derived from the classical truss analogy and V_{c}
in-cludes all contributions from alternative mechanisms. In a similar
vein, steel ibers contribute a third term to the equilibrium equation:

### (3)

### V

u### = V

c### + V

s### + V

fwhere V_{c} is the shear force resisted by alternative mechanisms in
a reinforced concrete beam *without *ibers.

A fourth term, Vr, represents the negative contribution of reverse

load-ing under identical conditions. Thus, the equilibrium condition becomes

### (4)

### V

u### = V

c### + V

s### + V

f### - V

r### Figure 4 – Stirrup stress values

### for the 40 MPa beams

### Figure 5 – Stirrup stress values

### for the 60 MPa beams

### Figure 6 – Stirrup stress values

### for the 80 MPa beams

rate of increase approximately follows what is predicted by the classical truss analogy.

However, the stirrup tensions were never *higher* than the
classi-cal truss analogy prediction, even for beams subjected to reverse
loadings. This fact conirms the point that some alternative mecha
-nisms are at work even if the concrete compressive chord (arch
action) and aggregate interlock are irrelevant. The longitudinal
re-inforcement pin effect (dowel action) is likely important.

Within each series, the type of loading and presence of ibers clearly had inluenced the load-stress behavior of the beam. Fig-ures [4], [5], and [6] fulill expectations that the beam free of ibers subjected to reverse loading (BC00I) are closer to approximate the classical truss model than the beam free of ibers subjected to nor-mal loading (BC00N). Furthermore, the beam with ibers subjected to normal loading (BC30N) has less similarity to the classical truss model than beam BC00N. These observations conirm that loading reversion has an unfavorable effect on the beam’s ultimate shear load, while the ibers bring a favorable contribution.

Likewise, the addition of ibers restores some supporting capacity on reverse-loaded beams. Indeed, the stirrup stress values of beams with ibers subjected to reverse loading (BC30I) were similar to those ob-served in beams without ibers subjected to normal loading (BC00N). Finally, the shear strength of a concrete beam subjected to reverse loading is lower than a similar beam subjected to normal loading. This decrease is important, but not large enough to match the val-ues predicted by the classical truss analogy.

Figure [7] shows that normally loaded beams with higher compres
-sive strengths have higher V_{c} contributions. Among beams subjected
to reverse loading, however, this effect was not evident (Figure [8]).

Table [2] shows the ultimate shear force contributions (Vu, Vc, Vf

and V_{r}) for each beam. V_{s} and V_{c }are calculated using equation 1
and equation 2 respectively. Vr, is the difference between beams of

type “N” and type “I”. In the same way, Vf is the ultimate shear force

difference between similar beams with and without ibers. The favorable contribution of ibers is comparable to Vc in all cases.

On average, Vf is 21% of Vc for beams subjected to normal loading

and 26% of Vc for beams subjected to reverse loading.

The unfavorable contribution of loading inversion (V_{r}) is 28% of V_{c}
for beams without ibers, and 23% of Vc for iber-reinforced beams.

**3.3 Ultimate shear strength – iber-reinforcement **

**3.3 Ultimate shear strength – iber-reinforcement**

**concrete beams**

**concrete beams**

This section compares the experimental values of Vu (=Pu/2) for

beams with ibers to three expressions proposed in the literature (Al-Taán and Al-Feel [1]; Swamy et al. [20]; Sharma [17]). The expression proposed by Al-Ta’an and Al-Feel [1] is based on a regression analysis of experimental data for 89 beams. Their result is reproduced below.

### (6)

*f*

*f*
*f*

*f*

_{D}

_{D}

*L*

*k*

### v

### 9

### 5

### .

### 8

### =

### n

### (MPa)

where *k* is a factor relecting the iber’s shape. For hooked ibers
such as those used in the present research, Al-Ta’an and Al-Feel
[1] propose the value *k* = 1.2.

### Figure 7 – Stirrup stress values

Swamy et al. [21] evaluated the contribution of ibers in terms of the average iber-matrix interfacial bond stress. Their result is

### (7)

### V

f### = 0.37

### t

### V

f_{D}

### Lf

f

### (MPa)

The value of 4.15 N/mm2_{ was adopted for the parameter t in the }

absence of speciic pullout tests on the iber-reinforced concrete used in this investigation.

Finally, Sharma [17] derived empirical formula for the shear strength of iber-reinforced concrete beams:

### (8)

### V

c### + V

f### = k´ f

t### ´

## (

### d

_{a}

## )

0.25### (MPa)

and

### (9)

### V

c### = 0.166 .

**√**

### f

c´where κ´ is equal to 0.667 because ƒ´_{t} is the indirect tensile
strength determined by splitting tension tests.

Table [3] compares Vf. calculated with the three formulas proposed.

The formula of Swamy et al. [21] comes closer to the experimental data. The difference between the three models is clearly signiicant. According to the results of table 3, the concrete compressive

strength has little inluence on experimental values of Vf, .Swamy´s

[21] and Al-Taán and Al-Feel [1] proved these experimental results. It is interesting to note that amount of steel ibers, their aspect ratio, and their anchorage conditions were the same for all beams.

**3.4 Ultimate shear strength – concrete beams **

**3.4 Ultimate shear strength – concrete beams**

**subjected to reverse loading**

**subjected to reverse loading**

Current design procedures (ACI Committee 318 [2]) for concrete
beams subjected to reverse loading specify no contribution to the
ultimate shear strength from the so-called alternative mechanisms
(V_{c}=0). It means that beams subjected to reverse loading should
be designed according classical truss analogy (V_{c}=0).

Figures 5 to 8 show the stirrup stress values for the beams. At no

### Table 2 – Experimental shear force

### BEAM

### V

u### (kN)

### V

c### (kN)

### V -V

c r### (kN)

### V + V

c f### (kN)

### V + V - V

c f r### (kN)

### V

f### (kN)

### V

r### (kN)

### I80-BC00-N

### 55

### 33

### -

### -

### I80-BC00-I

### 46

### 24

### -

### 9

### I80-BC30-N

### 61

### 39

### 6

### -

### I80-BC30-I

### 54

### 32

### 8

### 7

### I60-BC00-N

### 54

### 32

### -

### -

### I60-BC00-I

### 45

### 23

### -

### 9

### I60-BC30-N

### 60

### 38

### 6

### -

### I60-BC30-I

### 54

### 32

### 9

### 6

### I40-BC00-N

### 49

### 27

### -

### -

### I40-BC00I

### 41

### 19

### -

### 8

### I40-BC30-N

### 56

### 34

### 7

### -

### I40-BC30-I

### 48

### 27

### 7

### 8

### Table 3 – Experimental and predicted results

### Beam

### Vf, (kN)

### EXPERIMENTAL

_{Al-Taan Swamy }

### PREDICTED

_{Sharma}

### I80-BC30N

### 6

### 2.7

### 3.7

### 6.2

### I80-BC30I

### 8

### 2.7

### 3.7

### 6.2

### I60-BC30N

### 6

### 2.7

### 3.7

### 3.1

### I60-BC30I

### 9

### 2.7

### 3.7

### 3.1

### I40-BC30N

### 7

### 2.7

### 3.7

### 0.8

time in these igures, the experimental stirrup tension exceed val
-ues predicted by the classical truss analogy (V_{c}=0). The
unfavor-able contribution of loading inversion (V_{r}) was signiicant (28% of
V_{c} on average for beam without ibers and 23% for iber-reinforced
beams) but quite distant to 100% (Vc=Vr).

Thus, the current shear design procedures are very conservative for the beams tested in this study with reverse loading. It´s worth noting that all the results presented in this paper refer to the shear strength behavior of beams with a speciic cross-section, 30 kg/m3

of steel ibers, and a particular load increment.

**4. Conclusions**

In this paper the effectiveness of steel ibers on the shear capac -ity of concrete beams with normal or reverse load was checked. The main variable investigated, in addition to the effect of steel ibers and reverse load, was the inluence of concrete compressive strength: 40 MPa, 60 MPa and 80 MPa.

A comparison between the experimental values of ultimate shear force and these values calculated by expressions proposed in the literature for beams with ibers showed that the formula of Swamy et al [21] comes closer to the experimental data.

According to the tests results, the concrete compressive strength has little inluence on the ultimate shear force for beams with i-bers. Swamy´s [20] and Al-Taán and Al-Feel [1] proved these ex -perimental results.

For beams with reverse loading tested in this research, the current
shear design procedures (V_{c}=0) showed very conservative. The
unfavorable contribution of loading inversion (V_{r}) was signiicant
(28% of Vc on average for beam without ibers and 23% for

iber-reinforced beams) but quite distant to 100% (Vc=Vr).

The results of this research showed that adding ibers can improve the shear capacity of load reverse beams. Concrete beams with steel ibers had shear strengths under reverse loading similar to the same beams loaded without iber.

At last, it is important to note that overall more experimental re-search has to be done to get more information about optimizing shear behavior of load reverse beams. The effects of several vari-ables involved in the shear behavior of concrete beams remain to be assessed, such as the longitudinal reinforcement ratio, the increment of reverse loading, the iber content of the concrete, the type of iber, and so on.

**5. References**

[01] Al-Ta’an, S.A., and Al-Feel, J.R. 1990. Evaluation of shear strength of ibre reinforced concrete beams. Cement Concrete Composites, 12(2): 87–94. [02] American ACI Committee 318, “Building Code

Requirements for Reinforced Concrete (ACI 318-08),” American Concrete Institute, Detroit. 2008.

[03] Araúz, A.C. 2000. Resistência ao Cisalhamento de Vigas de Concreto Armado Reforçado com Fibras de Aço. M.Sc. thesis, Structural Department, Civil Engineering Faculty, University of Campinas, Campinas, Brazil.

[04] Ashour, S.A., Hasanain, G.S., and Wafa, F.F. 1992. Shear behavior of high strength iber reinforced concrete beams. ACI Structural Journal, 89(2): 176–184. [05] Cucchiara, C., La Mendola, L., and Papia, M. 2004.

Effectiveness of stirrups and steel ibres as shear

reinforcement. Cement & Concrete Composites, 26: 777-786.

[06] Di Prisco, M., and Romero, J.A. 1996. Diagonal shear in thin-webbed reinforced concrete beams: ibre and stirrup roles at shear collapse. Magazine Concrete Research, 48(174): 59–76.

[07] Furlan Jr, S., and de Hanai, J.B. 1997. Shear behavior of iber reinforced concrete beams. Cement Concrete Composites, 19(4): 359–366.

[08] Leonhardt, F., and Walther, R. 1964. The Stuttgard shear tests 1961. Cement and Concrete Association, London, Translation 111.

[09] Mansur, M.A., Ong, K.C.G., and Paramasivan, P. 1986. Shear strength of ibrous concrete beams without stirrups. Journal of Structural Engineering, 112(9): 2066-2079.

[10] Mörsch, E. 1948. Teoria y práctica del hormigón armado. Barcelo, G. Gili.???

[11] Narayanan, R., and Darwish, I.Y.S. 1987. Use of steel as shear reinforcement. ACI Structural Journal, 84(3): 216-217.

[12] Narayanan, R., and Darwish, I.Y.S. 1988. Shear in mortar beams containing ibers and ly-ash. Journal of Structural Engineering, 114(1): 84–102.

[13] Noghabai, K. 2000. Beams of ibrous concrete in shear and bending: experiment and model. Journal Structure Engineering ASCE, 126(2): 243–251.

[14] Oh, B.H., and Lim, D.H. 1998. Shear behavior and shear analysis of reinforced concrete beams containing steel iber. Magazine of Concrete Research, 4(12): 283-291.

[15] Oliveira, M.A.A.M. 1999. Cisalhamento em vigas de concreto de alta resistência submetida a carregamento reverso. M.Sc. thesis, Structural Department, Civil Engineering Faculty, University of Campinas, Campinas, Brazil.

[16] Parra-Montesinos, G., Shear Strength of Beams with Deformed Steel Fibers. Concrete International, V. 28, No. 11, Nov., 2006, pp. 57-66.

[17] Paulay, T. 1971. Coupling beams of reinforced concrete shear walls. Journal of the Structural Division, 97(NST3): 2407-2419.

[18] Sharma, A.K. 1986. Shear-strengh of steel iber reinforced-concrete beams. ACI Structural Journal, 83(4): 624-628.

[19] Swamy, R.N., and Bahla, H.M. 1979. Inluence of iber reinforcement on the dowel resistance to shear. ACI Structural Journal, 76(2): 327–55.

[20] Swamy, R.N., and Balla, H.M. 1985. The effectiveness of steel ibers as shear reinforcement. Concrete International, (3): 35-40.

[21] Swamy, R.N., Jones, R., and Chiam, A.T.P. 1993. Inluence of steel ibres on the shear resistance of lightweight concrete T-beams. ACI Structural Journal, 90(1): 103–114.

[22] Tan, K.H., Murugappan, K., and Paramasivam, P. 1992. Shear behaviour of steel iber reinforced concrete beams. ACI Structral Journal, 89(6): 3–11. [23] Wang, N., Mindess, S., and Ko, K. 1996. Fibre